Issue Date 9/28/04
SECTION 03450Architectural Precast Concrete
PCI GUIDE SPECIFICATION FOR ARCHITECTURAL PRECASTCONCRETE
Guide Specification Development:
These Guide Specifications have been developed jointly by PCI,
Gensler and the American Institute ofArchitects (AIA), Master
Systems publishers of MASTERSPEC.
Guide SpecificationThis Guide Specification is intended to be
used as a basis for the development of an office
masterspecification or in the preparation of specifications for a
particular project. In either case this GuideSpecification must be
edited to fit the conditions of use. Particular attention should be
given to thedeletion of inapplicable provisions or inclusion of
appropriate requirements. Coordinate thespecifications with the
information shown on the contract drawings to avoid duplication or
Shaded portions are Notes to the Specification Writer.
SECTION 03450 ARCHITECTURAL PRECAST CONCRETE
This Section uses the term Architect. Change this term to match
that used to identify the designprofessional as defined in the
General and Supplementary Conditions. Verify that Section
titlesreferenced in this Section are correct for this Projects
Specifications; Section titles may have changed.
PART 1 GENERAL
1.1 RELATED DOCUMENTS
A. Drawings and general provisions of the Contract, including
General and Supplementary Conditionsand Division 1 Specification
Sections, apply to this Section.
A. This section includes the performance criteria, materials,
production, and erection of architecturalprecast concrete for the
entire project. The work performed under this section includes all
labor,material, equipment, related services, and supervision
required for the manufacture and erection ofthe architectural
precast concrete work shown on the contract drawings.
Adjust list below to suit Project. Delete paragraph below if not
listing type of units.
B. This Section includes the following:1. Architectural precast
concrete cladding and loadbearing units.
2. Insulated, architectural precast concrete units.3.
Brick-faced, architectural precast concrete units.4. Stone-faced,
architectural precast concrete units.
C. Related Sections include the following:
List below only products and construction that the reader might
expect to find in this Section but arespecified elsewhere. Other
sections of the specifications not referenced below, shall also
apply to theextent required for proper performance of this
1. Division 3 Section Cast-in-Place Concrete for placing
connection anchors in concrete.2. Division 3 Section
Glass-Fiber-Reinforced Concrete.3. Division 4 Section Dimension
Stone Cladding for furnishing stone facings and anchorages.4.
Division 4 Section Cast Stone for wet or dry cast stone facings,
trim, and accessories.5. Division 4 Section Unit Masonry Assemblies
for full-thickness brick facing, mortar, and anchorages.6. Division
5 Section Structural Steel for connection attachment to
structural-steel framing.7. Division 7 Section Water Repellents for
water-repellent finish treatments.8. Division 7 Section Sheet Metal
Flashing and Trim for flashing receivers and reglets.9. Division 7
Section Joint Sealants for elastomeric joint sealants and sealant
backings.10. Division 8 Section Aluminum Windows for windows set
into architectural precast concrete units and tiebacks for window
Retain paragraph below if a design reference sample has been
pre-approved and is available for review.
A. Design Reference Sample: Sample of approved architectural
precast concrete color, finish andtexture, pre-approved by
1.4 PERFORMANCE REQUIREMENTS
Retain this Article if delegating design responsibility for
architectural precast concrete units tofabricator. AIA Document
A201 requires Owner or Architect to specify performance and
A. Structural Performance: Provide architectural precast
concrete units and connections capable ofwithstanding design loads
within limits and under conditions indicated.
Retain paragraph above if placing design loads on Drawings;
retain paragraph and applicablesubparagraphs below if including
design loads here. Revise requirements below to suit Project,
andadd other performance and design criteria if applicable.
add other performance and design criteria if applicable.
B. Structural Performance: Provide architectural precast
concrete units and connections capable ofwithstanding the following
design loads within limits and under conditions indicated:
As a minimum dead loads include panel weight and the weight(s)
of the materials that bear on them.
1. Dead Loads: 2. Live Loads: 3. Wind Loads:
4. Seismic Loads:
5. Project Specific Loads:
Show locations here or on Drawings if different movement is
anticipated for different buildingelements. If preferred, change
deflection limits below to ratios such as L/300 for floors and
6. Design framing system and connections to maintain clearances
at openings, to allow for fabricationand construction tolerances,
to accommodate live load deflection, shrinkage and creep of
primarybuilding structure, and other building movements as follows:
a. Upward and downward movementof [1/2 inch (13 mm)] [3/4 inch (19
mm)] [1 inch (25 mm)].
Temperature value in first subparagraph below is suitable for
most of the U.S. based on assumeddesign temperature of 70 deg. F
(21 Deg. C). Revise to suit local conditions. Temperature data
isavailable from National Oceanic and Atmospheric Administration at
7. Thermal Movements: Provide for in-plane thermal movements
resulting from annual ambienttemperature changes of 80 deg F (27
deg C) . Use other values, greater orsmaller, whenever justified by
climatic conditions at the projectsite.
Delete paragraph below if fire resistance rating is not
required. Fire ratings depend on occupancy andbuilding construction
type, and are generally a building code requirement. When required,
fire-ratedproducts should be clearly identified on the design
8. Fire Resistance Rating: Select material and minimum
thicknesses to provide fire rating.
Delete paragraph below if window washing system is not
9. Window Washing System: Design panels for window washing
system indicated to resist forcestransmitted from window washing
equipment pull-out and horizontal shear. All design criteriafor
window washing system, including material and equipment, furnished
Retain paragraph below if stone faced precast concrete are used
10. Stone to Precast Anchorages: Provide anchors, as determined
through Owners or stonesupplier testing, in numbers, types and
locations as required to satisfy the performancecriteria specified,
but not less than the following.a. Minimum Anchorage Requirement:
Not less than 2 anchors per stone unit of less than 2
sq. ft. (0.19 sq. m) in area and 4 anchors per unit of less than
12 sq. ft. (1.1 sq. m) in areaand for units larger than 12 sq. ft.
(1.1 sq. m) in area, provide anchors spaced not morethan 24 inches
(600 mm) o.c. both horizontally and vertically, all located a
minimum of 6inches (150 mm) from stone edge.
Delete paragraph below if units are not used in parking
structure to resist impact load.
11. Vehicular Impact Loads: Design spandrel beams acting as
vehicular barrier for passenger cars toresist a single load of
6,000 lbs (26.7 kN) service load and 10,000 lbs (44.5 kN) ultimate
loadapplied horizontally in any direction to the spandrel beam,
with anchorages or attachmentscapable of transferring this load to
the structure. For design of these beams, assume the load toact at
a height of 18 inches (460 mm) above the floor or ramp surface on
an area not to exceed 1sq. ft. (305 mm_).
A. Product Data: For each type of product indicated. Retain
quality control records and certificates ofcompliance for 5 years
or period of warranty, whichever is greater.
B. Design Mixes: For each concrete mix along with compressive
strength and water-absorption tests.
C. Shop (Erection) Drawings: Detail fabrication and installation
of architectural precast concrete units.Indicate member locations,
plans, elevations, dimensions, shapes and cross sections.
Indicateaesthetic intent including joints, reveals, and extent and
location of each surface finish. Indicatedetails at building
corners.1. Indicate separate face and backup mix locations, and
thicknesses.2. Indicate welded connections by AWS standard symbols.
Detail loose and cast-in hardware, and
connections.3. Indicate locations, tolerances and details of
anchorage devices to be embedded in or attached to
structure or other construction.4. Indicate locations, extent
and treatment of dry joints if two-stage casting is proposed.5.
Indicate plans, and/or elevations showing unit location, and
sequence of erection for special
conditions.6. Indicate location of each architectural precast
concrete unit by same identification mark placed
on panel.7. Indicate relationship of architectural precast
concrete units to adjacent materials.8. Indicate locations and
details of brick units and joint treatment.9. Indicate locations
and details of stone facings, stone anchors, and joint widths.
10. Design Modifications:a. If design modifications are
necessary to meet the performance requirements and field
conditions, submit design calculations and drawings. Do not
adversely affect the appearance,durability or strength of units
when modifying details or materials and maintain the generaldesign
Retain subparagraph below if Performance Requirements Article is
retained. Delete or modify ifArchitect assumes or is required by
law to assume design responsibility.
11. Comprehensive engineering design [signed and sealed]
[certified] by the qualified professionalengineer responsible for
its preparation registered in the state in which the project is
located.Show governing panel types, connections, and types of
reinforcement, including specialreinforcement. Coordinate the
location, type, magnitude and direction of all imposed loadingsfrom
the precast system to the building structural frame with the
Engineer of Record.
Retain paragraph below if finishes, colors, and textures are
preselected, specified, or scheduled.
D. Samples: Design reference samples for initial verification of
design intent, approximately 12 by 12by 2 inches (300 by 300 by 50
mm), representative of finishes, color, and textures of
exposedsurfaces of architectural precast concrete units.1. When
back face of precast concrete unit is to be exposed, show samples
of the workmanship,
color, and texture of the backup concrete as well as the
E. Samples for each brick unit required, showing the full range
of color and texture expected. Supplysketch of each corner or
special shape with dimensions. Supply sample showingcolor and
texture of joint treatment.
Retain first paragraph below if procedures for welder
certification are retained in QualityAssurance Article.
F. Welding Certificates: Copies of certificates for welding
procedure specifications (WPS) andpersonnel.
Manufacturer should have a minimum of 2 years of production
experience in architectural precastconcrete work comparable to that
shown and specified, in not less than three projects of similar
scopewith the Owner or Architect determining the suitability of the
G. Qualification Data: For firms and persons specified in
Quality Assurance Article to demonstratetheir capabilities and
experience. Include list of completed projects with project names
andaddresses, names and addresses of architects and owners, and
other information specified.
Delete test reports below if not required.
H. Material Test Reports: From a qualified testing agency
indicating and interpreting test results ofthe following for
compliance with requirements indicated:
Retain paragraph above or below.
I. Material Certificates: Signed by manufacturers certifying
that each of the following itemscomplies with requirements.
Retain list below with either paragraph above. Edit to suit
1. Concrete materials.2. Reinforcing materials and prestressing
tendons.3. Admixtures.4. Bearing pads.5. Structural-steel shapes
and hollow structural sections.6. Insulation7. Brick units.8. Stone
17.6 QUALITY ASSURANCE
A. Erector Qualifications:
Erector should have a minimum of 2 years of experience in
architectural precast concrete workcomparable to that shown and
specified in not less than three projects of similar scope with the
owneror Architect determining the suitability of the experience.
The inclusion of erection in the precastconcrete contract should be
governed by local practices. See PCIs website www.pci.org for
1. A precast concrete erector Qualified by the
Precast/Prestressed Concrete Institute (PCI) prior tobeginning work
at the projectsite. Submit a current Certificate of Compliance
furnished by PCIdesignating qualification in [Category A
(Architectural Systems) for non-load-bearingmembers] [Category S2
(Complex Structural Systems) for load-bearing members].
Retain paragraph below if PCI-Qualified Erector is not available
2. An erector with a minimum of 2 years of experience who has
completed architectural precastconcrete work similar in material,
design, and extent to that indicated for this Project andwhose work
has resulted in construction with a record of successful in-service
performance andwho meets the following requirements:a. Retains a
PCI Certified Field Auditor, at erectors expense, to conduct a
field audit of a
project in the same category as this Project prior to start of
erection. Submits Erectors PostAudit Declaration.
b. The basis of the audit is the PCI Erectors Manual - Standards
and Guidelines for theErection of Precast Concrete Products MNL
B. Fabricator Qualifications: A firm that complies with the
following requirements and isexperienced in producing architectural
precast concrete units similar to those indicated for thisProject
and with a record of successful in-service performance.
1. Assumes responsibility for engineering architectural precast
concrete units to comply withperformance requirements. This
responsibility includes preparation of Shop Drawings
andcomprehensive engineering analysis by a qualified professional
Delete subparagraph above and below if Contractor is not
required to engage the services of aqualified professional engineer
and if submission of a comprehensive engineering analysis is
notretained in Submittals Article.
2. Professional Engineer Qualifications: A professional engineer
who is legally qualified topractice in jurisdiction where Project
is located and who is experienced in providingengineering services
of the kind indicated. Engineering services are defined as those
performedfor installations of architectural precast concrete that
are similar to those indicated for thisProject in material, design,
3. Participates in PCIs Plant Certification program at the time
of bidding and is designated a PCI-certified plant for Group A,
Category A1- Architectural Cladding and Load Bearing Units.
4. Has sufficient production capacity to produce required units
without delaying the Work.
Delete subparagraph below if fabricators are not required to be
registered with and approved byauthorities having jurisdiction.
List approved fabricators in Part 2 if required.
5. Is registered with and approved by authorities having
Retain first paragraph below if PCI Certification Program
provides quality assurance testing, andadditional quality assurance
testing is required. Testing agency is normally engaged by
C. Testing Agency Qualifications: An independent testing agency,
[acceptable to authorities havingjurisdiction] qualified according
to ASTM C 1077 and ASTM E 329 to conduct the testingindicated, as
documented according to ASTM E 548.
D. Design Standards: Comply with ACI 318 (ACI 318M) and the
design recommendations of PCIMNL 120, PCI Design Handbook Precast
and Prestressed Concrete, applicable to types ofarchitectural
precast concrete units indicated.
E. Quality-Control Standard: For manufacturing procedures and
testing requirements, quality- controlrecommendations, and
dimensional tolerances for types of units required, comply with PCI
MNL117, Manual for Quality Control for Plants and Production of
Architectural Precast ConcreteProducts.
Delete paragraph below if no welding is required. Retain Welding
Certificates Paragraph inSubmittals Article if paragraph below is
retained. AWS states that welding qualifications remain ineffect
indefinitely unless welding personnel have not welded for more than
six months or there is aspecific reason to question their
F. Welding: Qualify procedures and personnel according to AWS
D1.1, Structural Welding Code Steel; and AWS D1.4, Structural
Welding Code Reinforcing Steel.
Retain paragraph below if fire-rated units or assemblies are
required. Select either PCI MNL 124 orACI 216.1/TMS 0216.1 or
retain both if acceptable to authorities having jurisdiction.
ACI 216.1/TMS 0216.1 or retain both if acceptable to authorities
G. Calculated Fire-Test-Response Characteristics: Where
indicated, provide architectural precastconcrete units whose fire
resistance has been calculated according to [PCI MNL 124, Design
forFire Resistance of Precast Prestressed Concrete,] [ACI 216.1/TMS
0216.1, Standard Methodfor Determining Fire Resistance of Concrete
and Masonry Construction Assemblies,] and isacceptable to
authorities having jurisdiction.
PCI recommends review of preproduction sample panels or first
production unit. Revise size andnumber of sample panels to suit
H. Sample Panels: After sample approval and before fabricating
architectural precast concrete units,produce a minimum of two
sample panels approximately 16 square feet in size for review
byArchitect. Incorporate full scale details of architectural
features, finishes, textures, and transitionsin the sample
1. Locate panels where indicated or, if not indicated, as
directed by Architect.2. Damage part of an exposed-face surface for
each finish, color, and texture, and demonstrate
adequacy of repair techniques proposed for repair of surface
blemishes.3. After acceptance of repair technique, maintain one
sample panel at the manufacturers plant
and one at the projectsite in an undisturbed condition as a
standard for judging the completedWork.
4. Demolish and remove sample panels when directed.
PCI recommends production of finish and texture range samples
when color and texture uniformityconcerns could be an issue, the
Architect or precaster has not had previous experience with
thespecified mix and finish, or a large project has multiple
I. Range Samples: After sample panel approval and before
production fabriction of architecturalprecast concrete units,
produce a minimum of samples, approximately 16 squarefeet in size,
representing anticipated range of color and texture on projects
units. Following rangesample acceptance by the Architect, maintain
samples at the manufacturers plant as color andtexture
Delete paragraph and subparagraphs below if sample panels above
will suffice and the addedexpense of mockups is not required. If
retaining, indicate location, size, and other details ofmockups on
Drawings or by inserts. Revise wording if only one mockup is
J. Mockups: After sample approval but before production
fabrication of architectural precastconcrete units, construct full
sized mockups to verify selections made under sample Submittals
andto demonstrate aesthetic effects and qualities of materials and
execution. Mockup to berepresentative of the finished work in all
respects including glass, aluminum framing, sealants
andarchitectural precast concrete complete with all anchors,
connections, flashings, and joint fillers asaccepted on the final
shop drawings. Build mockups to comply with the following
requirements,using materials indicated for the completed work:
Revise or delete subparagraphs below to suit Project.
1. Build mockups in the location and of the size indicated or,
if not indicated, as directed byArchitect.
2. Notify Architect in advance of dates and times when mockups
will be constructed.3. Obtain Architects approval of mockups before
starting fabrication.4. In presence of Architect, damage part of an
exposed face for each finish, color, and texture, and
demonstrate materials and techniques proposed for repairs to
match adjacent undamagedsurfaces.
5. Maintain mockups during construction in an undisturbed
condition as a standard for judging thecompleted Work.
6. Demolish and remove mockups when directed.
Retain subparagraph below if mockups are erected as part of
building rather than separately andthe intention is to make an
exception to the default requirement in Division 1 Section,
QualityRequirements for demolishing and removing mockups.
7. Approved mockups may become part of the completed Work if
undamaged at the time ofSubstantial Completion.
Delete paragraph below if mockup above is to be used for Testing
K. Testing Mockup: Provide a single full sized mockup for
testing by others to the extent shown orindicated to simulate the
precast and window wall assembly. Refer to Division 8 WINDOW
ANDCURTAIN WALLS for requirements applicable to testing
architectural precast concrete systems inconjunction with windows
and window wall.
Delete below if Work of this Section is not extensive or complex
enough to justify a pre-installationconference. If retaining,
coordinate with Division 1.
L. Preinstallation Conference: Conduct conference at Project
site to comply with requirements inDivision 1 Section Project
Management and Coordination.
1.7 PRODUCT DELIVERY, STORAGE AND HANDLING
A. Store units with adequate dunnage and bracing and protect
units to prevent contact with soil,staining, and to prevent
cracking, distortion, warping or other physical damage.
B. Store units, unless otherwise specified, with non-staining,
C. Place stored units so identification marks are clearly
visible, and product can be inspected.
D. Deliver all architectural precast concrete units to the
project site in such quantities and at suchtimes to assure
compliance with the agreed project schedule and proper setting
sequence so as tolimit unloading units temporarily on the
E. Handle and transport units in a position consistent with
their shape and design in order to avoidexcessive stresses which
would cause cracking or damage.
F. Lift and support units only at designated points shown on the
G. Place non-staining resilient spacers of even thickness
between each unit.
H. Support units during shipment on non-staining shock absorbing
Coordination and responsibility for supply of items to be placed
on or in the structure to allow place-ment of precast concrete
units depends on type of structure and varies with local practice.
Clearlyspecify responsibility for supply and installation of
hardware. If not supplied by precast concretefabricator, supplier
should be listed and requirements included in related trade
sections. When thebuilding frame is structural steel, erection
hardware welded to the steel frame should be supplied andinstalled
as part of the structural steel. Ensure that type and quantity of
hardware items to be cast intoprecast concrete units for use of
other trades are specified or detailed in contract drawings
andfurnished to fabricator, with instructions, in a timely manner
in order not to delay the Work.
A. Furnish loose connection hardware and anchorage items to be
embedded in or attached to otherconstruction without delaying the
Work. Provide setting diagrams, templates, instructions,
anddirections, as required, for installation.
PART 2 PRODUCTS
Delete this Article unless naming fabricators. See PCIs magazine
Ascent or its Web sitewww.pci.org for current PCI-certified plant
A. Available Fabricators: Subject to compliance with
requirements, fabricators offering products thatmay be incorporated
into the Work include, but are not limited to, the following:
Retain above for nonproprietary or below for semiproprietary
specification. If above is retained,include procedure for approval
of other fabricators in Instructions to Bidders. Refer to Division
1Section Product Requirements.
B. Fabricators: Subject to compliance with requirements, provide
products by one of the following:1.
2.2 MOLD MATERIALS
A. Molds: Rigid, dimensionally stable, nonabsorptive material,
warp and buckle free, that willprovide continuous and true precast
concrete surfaces within fabrication tolerances indicated;
non-reactive with concrete and suitable for producing required
finishes.1. Mold-Release Agent: Commercially produced
liquid-release agent that will not bond with,
stain or adversely affect precast concrete surfaces and will not
impair subsequent surface orjoint treatments of precast
Delete below if form liners are not used. Form liners may be
used to achieve a special off-the-formfinish or to act as a
template for thin or half brick facings. Revise to add description
if particular formliner is selected.
finish or to act as a template for thin or half brick facings.
Revise to add description if particular formliner is selected.
B. Form Liners: Units of face design, texture, arrangement, and
configuration [indicated] [to matchprecast concrete design
reference sample]. Provide solid backing and form supports to
ensurethat form liners remain in place during concrete placement.
Use with manufacturersrecommended liquid-release agent that will
not bond with, stain, or adversely affect precastconcrete surfaces
and will not impair subsequent surface or joint treatments of
Delete below if not using retarder to help obtain exposed
C. Surface Retarder: Chemical set retarder capable of
temporarily delaying hardening of newlyplaced concrete mix to depth
of reveal specified.
2.3 REINFORCING MATERIALS
Select only one of the paragraphs and subparagraphs below to
suit steel reinforcement requirements.If retaining Performance
Requirements Article, consider reviewing selections with
A. Reinforcing Bars: ASTM A 615/A 615M, Grade 60 (Grade 420),
Retain paragraph below for reinforcement that is welded or if
added ductility is sought.
B. Low-Alloy-Steel Reinforcing Bars: ASTM A 706/A 706M,
The presence of chromate film on the surface of the galvanized
coating is usually visible as a lightyellow tint on the surface.
ASTM B 201 describes a test method for determining the presence
ofchromate coatings. Use galvanizing where corrosive environment or
severe exposure conditionsjustify extra cost.
C. Galvanized Reinforcing Bars: ASTM A 767/A 767M, Class II zinc
coated, hot-dip galvanized andchromate wash treated after
fabrication and bending, as follows:
Select type of reinforcement to be galvanized from subparagraph
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade
420)] [ASTM A 706/A706M], deformed.
Use epoxy coating where corrosive environment or severe exposure
conditions justify extra cost.ASTM A775 is a bendable coating while
ASTM A934 is a non-bendable coating.
D. Epoxy-Coated Reinforcing Bars: ASTM A 775/A 775M or ASTM A
934/A 934M, as follows:
Select type of reinforcement to be epoxy coated from
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade
420)] [ASTM A 706/A706M], deformed.
E. Steel Bar Mats: ASTM A 184/A 184M, assembled with clips, as
Select type of reinforcement for mat fabrication from
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade 420)
[ASTM A 706/A706M], deformed bars.
Select only one of the paragraphs and subparagraphs below to
suit steel reinforcement requirements.If retaining Performance
Requirements Article, consider reviewing selections with
F. Plain-Steel Welded Wire Reinforcement: ASTM A 185, fabricated
from [as-drawn] [galvanizedand chromate wash treated] steel wire
into flat sheets.
G. Deformed-Steel Welded Wire Reinforcement: ASTM A 497, flat
H. Epoxy-Coated-Steel Welded Wire Reinforcement: ASTM A 884/A
884M Class A coated, [plain][deformed], flat sheet, [Type 1
bendable coating] [Type 2 non-bendable coating].
I. Supports: Suspend reinforcement from back of mold or use
bolsters, chairs, spacers, and otherdevices for spacing,
supporting, and fastening reinforcing bars and welded wire
reinforcement inplace according to PCI MNL 117.
2.4 PRESTRESSING TENDONS
Retain this Article if precast concrete units will be
prestressed, either pre-tensioned or post-tensioned. ASTM A 416/A
416M establishes low-relaxation strand as the standard
A. Prestressing Strand: ASTM A 416/A 416M, Grade 270 (Grade
1860), uncoated, 7-wire, low-relaxation strand.
B. Unbonded Post-Tension Strand: ASTM A416/A416M with corrosion
inhibitor conforming toASTM D1743, Grade 270 (Grade 1860), 7-wire,
low-relaxation strand with polypropylene conduitsheath.
2.5 CONCRETE MATERIALS
Delete materials below not required. Revise to suit Project.
A. Portland Cement: ASTM C150, Type I or III.
Select portland cement color from options in subparagraph below.
Mixing with white cement willimprove color uniformity of gray
cement. White cement has greater color consistency than graycement
and should be used for pastel colors. For darker colors, the
variations of gray cement haveless effect on the final color
1. For surfaces exposed to view in finished structure, use
[gray] [and] [white], same type, brand,and mill source throughout
the precast concrete production.
2. Standard gray Portland cement may be used for non-exposed
B. Supplementary Cementitious Materials.
Select mineral or cementitious admixtures from four paragraphs
below. Where appearance is animportant factor, it is recommended
that fly ash, silica fume and ground slag not be permitted.
1. Fly Ash Admixture: ASTM C 618, Class C or F with maximum loss
on ignition of 3 percent.2. Metakaolin Admixture: ASTM C 618, Class
N.3. Silica Fume Admixture: ASTM C 1240 with optional chemical and
physical requirement.4. Ground Granulated Blast-Furnace Slag: ASTM
C989, Grade 100 or 120.
ASTM C 33 limits deleterious substances in coarse aggregate
depending on climate severity and in-service location of concrete.
Class 5S is the most restrictive designation for architectural
concreteexposed to severe weathering. PCI MNL 117 establishes
stricter limits on deleterious substances forfine and coarse
B. Normal-Weight Aggregates: Except as modified by PCI MNL 117,
ASTM C 33, with coarseaggregates complying with Class 5S. Provide
and stockpile fine and coarse aggregates for eachtype of exposed
finish from a single source (pit or quarry) for entire project.
Revise subparagraph below and add descriptions of selected
coarse- and fine-face mix aggregatecolors, sizes, and sources if
1. Face-Mix Coarse Aggregates: Selected, hard, and durable; free
of material that reacts withcement or causes staining; to match
selected finish sample.
Retain one option from first subparagraph below or insert
gradation and maximum aggregate size ifknown. Fine and coarse
aggregates are not always from same source.
a. Gradation: [Uniformly graded] [Gap graded] [To match design
2. Face-Mix Fine Aggregates: Selected, natural or manufactured
sand of the same material ascoarse aggregate, unless otherwise
approved by Architect.
Delete paragraph below when architectural requirements dictate
that face-mix be used throughout.
C. Backup Concrete Aggregates: ASTM C33 or C330.
Lightweight aggregates in a face-mix are not recommended in cold
or humid climates (if exposed tothe weather) unless their
performance has been verified by tests or records of previous
satisfactoryusage in similar environments. If normal-weight
aggregates are used in face-mix, lightweightaggregates in backup
are not recommended due to bowing potential.
D. Lightweight Aggregates: Except as modified by PCI MNL 117,
ASTM C 330 with absorption lessthan 11 percent.
Delete first paragraph below if coloring admixture is not
required. Add color selection if known.E. Coloring Admixture: ASTM
C 979, synthetic or natural mineral-oxide pigments or colored
reducing admixtures, temperature stable and non-fading.
F. Water: Potable; free from deleterious material that may
affect color stability, setting, or strength ofconcrete and
complying with chemical limits of PCI MNL 117.
Delete paragraph below if air entrainment is not required. Air
entrainment should be required toincrease resistance to freezing
and thawing where environmental conditions dictate.
G. Air Entraining Admixture: ASTM C 260, certified by
manufacturer to be compatible with otherrequired admixtures.
Add types of chemical admixtures, if known, or limit types if
required. Water-reducing admixtures,Types A, E, and D, or a
high-range water reducer, Type F, predominate.
H. Water-Reducing Admixture: ASTM C 494/C494M, Type A.
I. Retarding Admixture: ASTM C 494/C494M, Type B.
J. Water-Reducing and Retarding Admixture: ASTM C 494/C494M,
K. High-Range, Water-Reducing Admixture: ASTM C 494/C494M, Type
L. High-Range, Water-Reducing and Retarding Admixture: ASTM C
494/C494M, Type G.
M. Plasticizing Admixture for Flowable Concrete: ASTM C
N. Admixtures containing calcium chloride, or more than 0.15
percent chloride ions or other salts byweight of admixture are not
2.6 STEEL CONNECTION MATERIALS
Edit this Article to suit Project. Add other materials as
A. Carbon-Steel Shapes and Plates: ASTM A 36/A 36M except
silicon (Si) content in the range of 0to 0.03% or 0.15 to 0.25% for
materials to be galvanized. Steel with chemistry conforming to
theformula Si + 2.5P < 0.09 is also acceptable.
B. Carbon-Steel Headed Studs: ASTM A 108, Grades 1018 through
1020, cold finished and bearingthe minimum mechanical properties
for studs as indicated under MNL 117, Table 3.2.3.; AWSD1.1, Type A
or B, with arc shields.
C. Carbon-Steel Plate: ASTM A 283/A 283M.
D. Malleable Iron Castings: ASTM A 47/A 47M. Grade 32510 or
E. Carbon-Steel Castings: ASTM A 27/A 27M, Grade U-60-30 (Grade
F. High-Strength, Low-Alloy Structural Steel: ASTM A 572/A 572M
except silicon (Si) content inthe range of 0 to 0.03% or 0.15 to
0.25% for materials to be galvanized. Steel with
chemistryconforming to the formula Si + 2.5P < 0.09 is also
G. Carbon-Steel Structural Tubing: ASTM A 500, Grade B.
H. Wrought Carbon-Steel Bars: ASTM A 675/A 675M, Grade 65 (Grade
I. Deformed-Steel Wire or Bar Anchors: ASTM A 496 or ASTM A
ASTM A 307 defines the term studs to include stud stock and
J. Carbon-Steel Bolts and Studs: ASTM A 307, Grade A (ASTM F
568M, Property Class 4.6)carbon-steel, hex-head bolts and studs;
carbon-steel nuts (ASTM A563/A563M, Grade A); and flat,unhardened
steel washers (ASTM F844).
High-strength bolts are used for friction-type connections
between steel members and are notrecommended between steel and
concrete since concrete creep and crushing of concrete during
bolttightening reduce effectiveness.
K. High-Strength Bolts and Nuts: ASTM A 325/A 325M or ASTM
A490/A490M, Type 1, heavy hexsteel structural bolts, heavy hex
carbon-steel nuts, (ASTM A563/A563M) and hardened carbon-steel
washers (ASTM F436/F436M).
Retain paragraph and subparagraph below if galvanized finish is
required. Revise locations ofgalvanized items if required. Field
welding should generally not be permitted on galvanizedelements,
unless the galvanizing is removed or acceptable welding procedures
are submitted. Hot-dip galvanized finish provides greater corrosion
resistance than electrodeposited zinc coating.Electrodeposition is
usually limited to threaded fasteners.
L. Finish: For exterior steel items and items indicated for
galvanizing, apply zinc coating by [hot-dipprocess according to
ASTM A 123/A 123M, after fabrication, or ASTM A 153/A 153M,
asapplicable] [electrodeposition according to ASTM B 633, SC 3,
Type 1and 2].1. Galvanizing Repair Paint: High-zinc-dust-content
paint with dry film containing not less than
94 percent zinc dust by weight, and complying with DOD-P-21035A
or SSPC-Paint 20.
Retain paragraph below if paint finish is required. Revise
locations of priming, if required. MPI 79(FS TT-P-664) in first
option below provides some corrosion protection while SSPC-Paint
25,without topcoating, provides minimal corrosion protection.
M. Shop-Primed Finish: Prepare surfaces of non-galvanized steel
items, except those surfaces to beembedded in concrete, according
to requirements in SSPC-SP 1 followed by SSPC-SP 3 and shop-apply
[lead- and chromate-free, rust inhibitive primer, complying with
performancerequirements in MPI 79] [SSPC-Paint 25] according to
N. Welding Electrodes: Comply with AWS standards.
2.7 STAINLESS-STEEL CONNECTION MATERIALS
Delete this Article if not required. Use when resistance to
staining merits extra cost in parkingstructures and other high
moisture or corrosive areas.
A. Stainless-Steel Plate: ASTM A 666, Type 304, of grade
suitable for application.
B. Stainless-Steel Bolts and Studs: ASTM F 593, alloy 304 or
316, hex-head bolts and studs;stainless-steel nuts; and flat,
stainless steel washers. Lubricate threaded parts of stainless
steelbolts with an anti-seize thread lubricant during assembly.
C. Stainless-Steel Headed Studs: ASTM A 276 and bearing the
minimum mechanical properties forstuds as indicated under MNL 117,
2.8 BEARING PADS AND OTHER ACCESSORIES
Delete this Article if not applicable. Choice of bearing pad can
usually be left to fabricator;coordinate selection with structural
engineer if required.
A. Provide bearing pads for architectural precast concrete units
as follows:1. Elastomeric Pads: AASHTO M 251, plain, vulcanized,
100 percent polychloroprene
(neoprene) elastomer, molded to size or cut from a molded sheet,
50 to 70 Shore A durometeraccording to ASTM D2240, minimum tensile
strength 2250 psi (15.5 MPa) per ASTM D 412.
2. Random-Oriented, Fiber-Reinforced Elastomeric Pads:
Preformed, randomly orientedsynthetic fibers set in elastomer.
Surface hardness of 70 to 90 Shore A durometer according toASTM
D2240. Capable of supporting a compressive stress of 3000 psi (20.7
MPa) with nocracking, splitting or delaminating in the internal
portions of the pad. Test one specimen foreach 200 pads used in the
3. Cotton-Duck-Fabric-Reinforced Elastomeric Pads: Preformed,
horizontally layered cotton-duck fabric bonded to an elastomer.
Surface hardness of 80 to 100 Shore A durometeraccording to ASTM
D2240. Conforming to Division II, Section 18.10.2 of AASHTO
LRFDBridge Design Specifications, or Military Specification,
4. Frictionless Pads: Tetrafluoroethylene (teflon), glass-fiber
reinforced, bonded to stainless ormild-steel plates, of type
required for in-service stress.
5. High-Density Plastic: Multimonomer, nonleaching, plastic
Select material from options in paragraph below or add another
material to suit Project. Coordinatewith counterflashing materials
B. Reglets: [PVC extrusions.] [Stainless steel, Type 302]
[Copper] [Reglets and flashing arespecified in Division 7 Section
Sheet Metal Flashing and Trim.] felt or fiber filled or coverface
opening of slots.
C. Accessories: Provide clips, hangers, plastic or steel shims,
and other accessories required to installarchitectural precast
2.9 GROUT MATERIALS
Add other proprietary grout systems to suit Project. Show
locations of each grout here or onDrawings if more than one type is
A. Sand-Cement Grout: Portland Cement, ASTM C 150, Type I, and
clean, natural sand, ASTM C144, or ASTM C 404. Mix at ratio of 1
part cement to 2-1/2 parts sand, by volume, with minimumwater
required for placement and hydration.
Retain paragraph below if nonshrink grout is required or if
cement-grout shrinkage could causestructural deficiency. For
critical installations, require manufacturer to provide field
B. Nonmetallic, Nonshrink Grout: Premixed, nonmetallic,
noncorrosive, nonstaining grout containingselected silica sands,
portland cement, shrinkage-compensating agents, plasticizing and
water-reducing agents, complying with ASTM C 1107, Grade A for
drypack and Grades B and C forflowable grout and of a consistency
suitable for application within a 30-minute working time.
C. Epoxy-resin grout: Two-component mineral-filled epoxy-resin:
ASTM C881 of type, grade, andclass to suit requirements.
2.10 THIN AND HALF BRICK UNITS AND ACCESSORIES
Retain this Article if specifying thin veneer brick-faced
precast concrete panels. Type TBX brickunits feature the tightest
dimensional tolerances but may be too dimensionally variable to
fitsecurely within form liner templates. Pre-select brick and name
prior to bid or establish set costallowance. If full-size brick
units are required, use Division 4 Section Unit Masonry
A. Thin or Half Brick Units: ASTM C216, Type FBX or ASTM C 1088,
Grade Exterior, Type TBX,[not less than _ inch (13 mm)] [3/4 inch
(19 mm)] [1 inch (25 mm)] thick with a tolerance ofplus or minus
1/16 inch (1.59 mm) and as follows:1. Face Size: Standard, 2-1/4
inches (57 mm) high by 8 inches (203 mm) long.2. Face Size:
Modular, 2-1/4 inches (57 mm) high by 7-1/2 to 7-5/8 inches (190 to
194 mm) long.3. Face Size: Engineer Modular, 2-3/4 to 2-13/16
inches (70 to 71 mm) high by 7-1/2 to 7-5/8
inches (190 to 194 mm) long.4. Face Size: Closure Modular, 3-1/2
to 3-5/8 inches (89 to 92 mm) high by 7-1/2 to 7-5/8 inches
(190 to 194 mm) long.5. Face Size: Utility, 3-1/2 to 3-5/8
inches (89 to 92 mm) high by 11-1/2 to 11-5/8 inches (292 to
295 mm) long.6. [Where shown to match existing,] provide face
brick matching color, texture, and face size
of existing adjacent brickwork.a.
Select from subparagraphs above face sizes with equivalent
metric dimensions or fromsubparagraphs below for products
manufactured to metric face sizes. If retaining below,
verifyavailability of sizes.
7. Face Size: Metric modular, 57 mm high by 190 mm long.8. Face
Size: Metric engineer, 70 mm high by 190 mm long.9. Face Size:
Metric closure, 90 mm high by 190 mm long.10. Face Size: Metric
utility, 90 mm high by 290 mm long.
Show details on Drawings of special conditions and shapes if
11. Special Shapes: Include corners, edge corners, and end edge
Thin brick units with higher rates of absorption than values in
first subparagraph below should bewetted before placing concrete to
improve bond. Before retaining paragraph, verify that thin
brickselected complies with requirements.
12. Initial Rate of Absorption: Less than 30g/30 sq. in.
(30g/194 sq. cm.) per minute when testedper ASTM C 67.
13. Efflorescence: Provide brick that has been tested according
to ASTM C 67 and is rated noteffloresced.
Delete subparagraph below if surface-colored brick is not
14. Surface Coloring: Brick with surface coloring, other than
flashed or sand-finished brick, shallwithstand 50 cycles of
freezing and thawing per ASTM C 67 with no observable difference
inthe applied finish when viewed from 10 feet (3 m).
Options in subparagraph below are examples of descriptive
requirements for appearance where aproprietary specification cannot
be used. If approving a color range for brick, view 100 square
feetof loose bricks or a completed building. Edit to suit Project
or delete if brick is specified by productname.
15. Face Color and Texture: [Match Architects samples] [Medium
brown, wire cut] [Full-range red, sand molded] [Gray, velour].
Retain first subparagraph below, deleting inapplicable
descriptions if required.
16. Back Surface Texture: Scored, combed, wire roughened,
ribbed, keybacked or dovetailed.17. Available Products: Subject to
compliance with requirements, products that may be
incorporated into the Work include, but are not limited to, the
Retain subparagraph above for nonproprietary or subparagraph
below for semiproprietarySpecification. Refer to Division 1 Section
Materials and Equipment.
18. Products: Subject to compliance with requirements, provide
one of the following:
Refer to American National Standards Institute (ANSI) A 137.1
for the commonly available sizesand shapes, physical properties,
the basis for acceptance and methods of testing.
B. Glazed and Unglazed Ceramic Tile Units: ANSI A 137.1 [not
less than 3/8 inch (10 mm)]1. Body of glazed tile shall have a
water absorption of less than 3 percent using ASTM C373.2.
Manufacturer shall warrant materials as frost-resistant.3. Glazed
units shall conform to ASTM C126.
C. Architectural Terra Cotta Units: Comply with requirements of
Architectural Terra Cottamanufacturers standards for the
Retain paragraph below if mortar setting brick unit joints
before placing precast concrete mix.
D. Setting Mortar: Portland cement, ASTM C 150, Type I, and
clean, natural sand, ASTM C 144.Mix at ratio of 1 part cement to 4
parts sand, by volume, with minimum water required
Delete paragraph and subparagraphs below if not filling thin
brick unit joints with pointing groutafter precast concrete panel
E. Latex-Portland Cement Pointing Grout: ANSI A118.6 and as
Select one or both types of grout from first two subparagraphs
1. Dry-grout mixture, factory prepared, of portland cement,
graded aggregate, and dry,redispersible, ethylene-vinyl-acetate
additive for mixing with water; uniformly colored.
2. Commercial portland cement grout, factory prepared, with
liquid styrene-butadiene rubber oracrylic-resin latex additive;
3. Colors: [As indicated by manufacturers designations] [Match
Architects samples] [Asselected by Architect from manufacturers
F. Setting Systems
Retain paragraphs below if thin brick, ceramic tile, or full
brick will be laid after casting of panel.
1. Thin brick and Ceramic Tile Units: [Dry-Set Mortar: ANSI
A118.1] [Latex-Portland Cement Mortar: ANSI A 118.4]2. Full Brick
Units: Install dovetail slots in precast:
not less than 0.5 mm thick, felt or fiber filled or cover face
opening of slots. Attach brick units with wire anchors, ASTM A82 or
B227, Grade 30HS not less than 3/16 inch (W2.8) in diameter and
hooked on one end and looped through a 7/8 in. (25 mm) wide,
12-gage (2.68 mm) steel sheet bent over the wire with dovetail on
2.11 STONE MATERIALS AND ACCESSORIES
Retain this Article if stone facing is required. Material,
fabrication, and finish requirements areusually specified in
Division 4 Section Dimension Stone Cladding. Replace first
paragraph belowwith stone requirements, if preferred.
usually specified in Division 4 Section Dimension Stone
Cladding. Replace first paragraph belowwith stone requirements, if
A. Stone facing for architectural precast concrete is specified
in Division 4 Section Dimension StoneCladding.1. Tolerance of
length and width of +0, -1/8 inch (+0, -3mm).
Anchors are generally supplied by stone fabricator or, in some
cases, by precaster. Specify supplier.Anchors may be toe-in,
toe-out, or dowels.
B. Anchors: Stainless steel, ASTM A 666, Type 304, of temper and
diameter required to supportloads without exceeding allowable
Grommets will usually be required if filling dowel holes with
1. Fit each anchor leg with 60 durometer neoprene grommet collar
of width at least twice thediameter and of length at least five
times the diameter of the anchor.
C. Sealant Filler: ASTM C 920, low-modulus, multicomponent,
nonsag urethane sealant complyingwith requirements in Division 7
Section Joint Sealants and that is nonstaining to stone
Dowel hole filling is used to prevent water intrusion into stone
and future discoloration at anchorlocations. Retain paragraph above
for a flexible filler or paragraph below for a rigid filler.
D. Epoxy Filler: ASTM C 881, 100 percent solids, sand filled
non-shrinking, non -staining of type,class, and grade to suit
E. Bond Breaker:1. Preformed, compressible, resilient,
nonstaining, nonwaxing, closed-cell polyethylene foam pad,
nonabsorbent to liquid and gas, 1/8 inch (3.2 mm) thick.2.
Polyethylene sheet, 6 to 10 mil thick.
2.12 INSULATED PANEL ACCESSORIES
Retain this Article if insulated, architectural precast concrete
panels are required. State desiredminimum aged R-value or thickness
required, or both. Select insulation material from one of thethree
following paragraphs; if using more then one type identify
A. Expanded-Polystyrene Board Insulation: Rigid, cellular
polystyrene thermal insulation complyingwith ASTM C578 formed by
expansion of polystyrene base resin; ; with R-value of and
thickness of .
B. Extruded-Polystyrene Board Insulation: Rigid cellular
polystyrene thermal insulation complyingwith ASTM C578 formed from
polystyrene base by an extrusion process; ; with R-value of and
thickness of .
C. Polyisocyanurate Board Insulation: Rigid, cellular
polyisocyanurate thermal insulation; complying with ASTM C 591;
square edged; with R-value of and thickness of .
Select wythe connectors from paragraph below.
D. Wythe Connectors: , , , , , manufactured to connect wythes of
precast concrete panels.
2.13 CONCRETE MIXES
A. Prepare design mixes to match Architects sample for each type
of concrete required.
Revise subparagraph below if fly ash, blast furnace slag, or
silica fume are not permitted. Revisepercentage to suit
1. Limit use of fly ash and granulated blast-furnace slag to 20
percent replacement of portland cement by weight; metakaolin and
silica fume to 10 percent of portland cement by weight.
B. Design mixes may be prepared by a qualified independent
testing agency or by qualified precastplant personnel at
architectural precast concrete fabricators option.
C. Limit water-soluble chloride ions to the maximum percentage
by weight of cement permitted byACI 318 (ACI 318M) or PCI MNL 117
when tested in accordance with ASTM C1218/C1218M.
Architectural precast concrete units may be manufactured with a
separate architectural face mixand a structural backup mix. Face
and backup mixes should have similar shrinkage and
expansioncoefficients. Similar water-cementitious materials ratios
and cement-aggregate ratios arerecommended to limit bowing or
D. Normal-Weight Concrete Face and Backup Mixes: Proportion
mixes by either laboratory trialbatch or field test data methods
according to ACI 211.1, with materials to be used on project,
toprovide normal-weight concrete with the following properties:
Retain subparagraph below or revise to suit Project.
Higher-strength mixes may be available; verifywith fabricators.
1. Compressive Strength (28 Days): 5000 psi (34.5 MPa).
A water-cementitious materials ratio of 0.40 to 0.45 is usual
for architectural precast concrete.Lower ratios may be possible
with use of high-range water reducers. Revise ratio as
2. Maximum Water-Cementitious Materials Ratio: 0.45.
Water absorption indicates susceptibility to weather staining.
The limit in paragraph below,corresponding to 6 percent by weight,
is suitable for average exposures. Different parts of a singlepanel
cannot be produced with different absorptions. Verify that
fabricator can produce units withlower water absorption because
special consolidation techniques to increase concrete density
E. Water Absorption: 6 percent by weight or 14 percent by
volume, tested according to PCI MNL117.
Lightweight backup mixes must be compatible with normal-weight
face mixes to minimize bowingor warping. Retain lightweight
concrete backup mixes if required or as an option if
satisfactorydurability and in-service performance are verified by
F. Lightweight Concrete Backup Mixes: Proportion mixes by either
laboratory trial batch or field testdata methods according to ACI
211.2, with materials to be used on Project, to provide
lightweightconcrete with the following properties:
Retain subparagraph below or revise to suit Project.
Higher-strength mixes may be available; verifywith fabricators.
1. Compressive Strength (28 Days): 5000 psi (34.5 MPa).
Increase or decrease unit weight as required. Coordinate with
lightweight-aggregate supplier andarchitectural precast concrete
fabricator. Lightweight concretes with lightweight and
normal-weightaggregate in mix will usually be heavier than unit
2. Unit Weight: Calculated equilibrium unit weight of 115
lb/cu.ft. (1842 kg/cu.m), plus or minus3 lb/cu.ft. (48 kg/cu.m),
according to ASTM C 567.
G. Add air-entraining admixture at manufacturers prescribed rate
to result in concrete at point ofplacement having an air content
complying with PCI MNL 117.
H. When included in design mixes, add other admixtures to
concrete mixes according tomanufacturers written instructions.
2.14 MOLD FABRICATION
A. Molds: Accurately construct molds, mortar tight, of
sufficient strength to withstand pressures dueto concrete-placement
and vibration operations and temperature changes and for
prestressing anddetensioning operations. Coat contact surfaces of
molds with release agent before reinforcement isplaced. Avoid
contamination of reinforcement and prestressing tendons by release
Delete form liners unless needed to produce exposed surface
1. Place form liners accurately to provide finished surface
texture indicated. Provide solidbacking and supports to maintain
stability of liners during placing of concrete. Coat form linerwith
B. Maintain molds to provide completed architectural precast
concrete units of shapes, lines, anddimensions indicated, within
fabrication tolerances specified.1. Form joints are not permitted
on faces exposed to view in the finished work.
Select one option from below; show details on Drawings or revise
description to add dimensions.Sharp edges or corners of precast
concrete units are vulnerable to chipping.
2. Edge and Corner Treatment: Uniformly [chamfered]
2.15 THIN AND HALF BRICK FACINGS
Retain this Article if using thin or half brick facings on
architectural precast concrete units.
A. Place form liner templates accurately to provide grid for
brick facings. Provide solid backing andsupports to maintain
stability of liners while placing bricks and during placing of
B. Securely place brick units face down into form liner pockets
and place precast concrete backingmix.
C. Clean faces and joints of brick facing.
2.16 STONE FACINGS
Retain this Article if stone facing is required. Refer to
Division 4 Section Dimensional StoneCladding for precast
A. Accurately position stone facings to comply with
requirements. Install spring clips, anchors,supports, and other
attachments indicated or necessary to secure stone in place. Set
stone facingsaccurately, in locations indicated on Shop Drawings.
Orient stone veining in direction indicated onShop Drawings. Keep
reinforcement a minimum of _ inch (19 mm) from the back surface
ofstone. Use continuous spacers to obtain uniform joints of widths
indicated and with edges andfaces aligned according to established
relationships and indicated tolerances. Ensure no passage ofprecast
matrix to stone surface.
B. See Division 7 Section Joint Sealants for furnishing and
installing sealant backings and sealantinto stone-to-stone joints
and stone-to-concrete joints. Apply a continuous sealant bead along
bothsides and top of precast panels at the stone/precast interface
using the bond breaker as a joint fillerback-up. Do not seal panel
Retain one of two subparagraphs below if sealing dowel holes.
Use sealant if a flexible filler isrequired; use epoxy if a rigid
filler is required.
1. Fill anchor holes with low modulus polyurethane sealant
filler and install anchors.2. Fill anchor holes with epoxy filler
and install anchors with _ inch (13 mm) long 60 durometer
elastomeric sleeve at the back surface of the stone.
PCI recommends preventing bond between stone facing and precast
concrete to minimize bowing,cracking, and staining of stone. Retain
one of two subparagraphs below.
3. Install 6 to 10 mil polyethylene sheet to prevent bond
between back of stone facing andconcrete substrate.
4. Install 1/8 inch (3 mm) polyethylene-foam bond breaker to
prevent bond between back of stonefacing and concrete substrate.
Maintain minimum projection requirements of stone anchorsinto
PCI recommends anchor spacing be determined prior to bidding.
Retain below if precaster is totest stone anchors for shear and
tension. ASTM E488 is preferred as ASTM C1354 does notinclude the
influence of the precast concrete backup.
C. Stone Anchor Shear and Tensile Testing: Engage a certified
testing laboratory acceptable to theArchitect to evaluate and test
the proposed stone anchorage system. Test for shear and
tensilestrength of proposed stone anchorage system in accordance
with ASTM E 488 or ASTM C 1354modified as follows:
1. Prior to testing, submit for approval a description of the
test assembly (including pertinent dataon materials), test
apparatus and procedures.
2. Test 12-by-12 inch (300 by 300 mm) samples of stone affixed
to testing apparatus throughproposed anchorages. Provide 2 sets of
6 stone samples each. One set for shear load testingand the other
set for tensile load testing.
3. Test stone anchors of the sizes and shapes proposed for the
installation.a. Test the assembly to failure and record the test
load at failure. Record the type of failure, anchor pull-out or
stone breakage, and any other pertinent information, in accordance
with the requirements of ASTM E 488. In addition, submit load
deflection curves of each test assembly.
D. Minimum Anchor Spacing: Anchor spaced not less than 6 inches
(152 mm) from an edge with notmore than 24 to 30 inches (610 to 760
mm) between anchors depending on the local building codeand wind
A. Cast-in Anchors, Inserts, Plates, Angles, and Other Anchorage
Hardware: Fabricate anchoragehardware with sufficient anchorage and
embedment to comply with design requirements.Accurately position
for attachment of loose hardware and secure in place during
precastingoperations. Locate anchorage hardware where it does not
affect position of main reinforcement orconcrete placement.1. Weld
headed studs and deformed bar anchors used for anchorage according
to AWS D1.1 and
AWS C5.4, Recommended Practices for Stud Welding.
Coordinate paragraph below with Division 5 Section Metal
Fabrications for furnishing andinstalling loose hardware items.
B. Furnish loose hardware items including steel plates, clip
angles, seat angles, anchors, dowels,cramps, hangers, and other
hardware shapes for securing architectural precast concrete units
tosupporting and adjacent construction.
C. Cast-in reglets, slots, holes, and other accessories in
architectural precast concrete units asindicated on contract
Delete first paragraph below if not applicable.
D. Cast-in openings larger than 10 inches (250 mm) in any
dimension. Do not drill or cut openings orprestressing strand
without approval of Architect.
E. Reinforcement: Comply with recommendations in PCI MNL 117 for
fabrication, placing, andsupporting reinforcement.
1. Clean reinforcement of loose rust and mill scale, earth, and
other materials that reduce ordestroy the bond with concrete. When
damage to epoxy coated reinforcing exceeds limitsspecified ASTM
A775/A775M repair with patching material compatible with coating
materialand epoxy coat bar ends after cutting.
2. Accurately position, support, and secure reinforcement
against displacement during concrete-placement and consolidation
operations. Completely conceal support devices to preventexposure
on finished surfaces.
3. Place reinforcing steel and prestressing strand to maintain
at least 3/4 -inch (19 mm) minimumconcrete cover. Increase cover
requirements for reinforcing steel to 1-1/2 inches (38 mm)when
units are exposed to corrosive environment or severe exposure
conditions. Arrange,space, and securely tie bars and bar supports
to hold reinforcement in position while placingconcrete. Direct
wire tie ends away from finished, exposed concrete surfaces.
4. Install welded wire reinforcement in lengths as long as
practicable. Lap adjoining pieces atleast one full mesh spacing and
wire tie laps, where required by design. Offset laps ofadjoining
widths to prevent continuous laps in either direction.
F. Reinforce architectural precast concrete units to resist
handling, transportation, and erectionstresses.
Delete paragraph and subparagraph below if prestressed
architectural precast concrete units are notrequired. Option to
prestress may be left to fabricator if objective is to aid handling
and to controlcracking of units during installation.
G. Prestress tendons for architectural precast concrete units by
either pretensioning or post-tensioningmethods. Comply with PCI MNL
Revise release or post-tensioning strength in subparagraph below
to an actual compressive strengthif required. A release strength as
low as 2500 psi (17.2 MPa) for normal-weight concrete and 3000psi
(20.7 MPa) for lightweight concrete is permitted.
1. Delay detensioning or post-tensioning of prestressed
architectural precast concrete units untilconcrete has reached its
indicated minimum design release compressive strength as
establishedby test cylinders cured under the same conditions as
2. Detension pretensioned tendons either by gradually releasing
tensioning jacks or by heat-cutting tendons, using a sequence and
pattern to prevent shock or unbalanced loading.
3. If concrete has been heat cured, detension while concrete is
still warm and moist to avoiddimensional changes that may cause
cracking or undesirable stresses.
4. Protect strand ends and anchorages with bituminous, zinc-rich
or epoxy paint to avoidcorrosion and possible rust spots.
H. Mix concrete according to PCI MNL 117 and requirements in
this Section. After concretebatching, no additional water may be
Retain paragraph below if a separate face mix is required or is
I. Place face mix to a minimum thickness after consolidation of
the greater of 1 inch (25 mm) or 1.5times the maximum aggregate
size, but not less than the minimum reinforcing cover as
indicatedon contract drawings.1. At the fabricators option either
of the following mix design/casting techniques may be used:
a. A single design mix throughout the entire thickness of
panel.b. Design mixes for facing and backup; using cement and
aggregates for each type as
indicated, for consecutive placement in the mold. Use cement and
aggregate specified forfacing mix, use cement and aggregate for
backup mix complying with criteria specified asselected by the
J. Place concrete in a continuous operation to prevent seams or
planes of weakness from forming inprecast concrete units. Comply
with requirements in PCI MNL 117 for measuring,
mixing,transporting, and placing concrete.1. Place backup concrete
to ensure bond with face mix concrete.
K. Thoroughly consolidate placed concrete by internal and/or
external vibration without dislocating ordamaging reinforcement and
built-in items, and minimize pour lines, honeycombing or entrapped
airon surfaces. Use equipment and procedures complying with PCI MNL
117.1. Place self-consolidating concrete without vibration in
accordance with PCI Interim Guidelines
for the Use of Self-Consolidating Concrete.
L. Comply with ACI 306.1 procedures for cold-weather concrete
M. Comply with ACI 305R recommendations for hot-weather concrete
O. Identify pickup points of architectural precast concrete
units and orientation in structure withpermanent markings,
complying with markings indicated on Shop Drawings. Imprint
orpermanently mark casting date on each architectural precast
concrete unit on a surface that will notshow in finished
P. Cure concrete, according to requirements in PCI MNL 117, by
moisture retention without heat or by accelerated heat curing using
low-pressure live steam or radiant heat and moisture. Cure units
until the compressive strength is high enough to ensure that
stripping does not have an effect on the performance or appearance
of the final product.
Q. Repair damaged architectural precast concrete units to meet
acceptability requirements of PCI MNL 117.
2.18 INSULATED PANEL CASTING
Delete this Article if integrally insulated panels are not
A. Cast and screed supported wythe over mold.
B. Place insulation boards, abutting edges and ends of adjacent
boards. Insert wythe connectors throughinsulation, and consolidate
concrete around connectors according to connector
C. Cast and screed top wythe to meet required finish.
2.19 FABRICATION TOLERANCES
A. Fabricate architectural precast concrete units straight and
true to size and shape with exposed edgesand corners precise and
true so each finished unit complies with PCI MNL 117 product
tolerances aswell as position tolerances for cast-in items.
Select paragraph above or paragraph and subparagraphs below.
Usually retain above unless tolerancesfor Project deviate from PCI
recommendations. PCI MNL 117 product tolerances, listed below,
arestandardized throughout the industry. For architectural trim
units such as sills, lintels, coping, cornices,quoins, medallions,
bollards, benches, planters, and pavers, tolerances are listed in
PCI MNL 135.
B. Fabricate architectural precast concrete units straight and
true to size and shape with exposed edgesand corners precise and
true so each finished unit complies with the following product
tolerances.1. Overall Height and Width of Units, Measured at the
Face Exposed to View: As follows:
a. 10 feet (3 m) or under, Plus or Minus 1/8 inch (3 mm).b. 10
to 20 feet (3 to 6 m), Plus 1/8 inch (3 mm), Minus 3/16 inch (5
mm).c. 20 to 40 feet (6 to 12 m), Plus or Minus 1/4 inch (6
mm).d.Each additional 10 feet (3 m), Plus or Minus 1/16 inch (1.5
2. Overall Height and Width of Units, Measured at the Face Not
Exposed to View: As follows:a. 10 feet (3 m) or under, Plus or
Minus 1/4 inch (6 mm).b. 10 to 20 feet (3 to 6 m), Plus _ inch (6
mm), Minus 3/8 inch (10 mm).c. 20 to 40 feet (6 to 12 m), Plus or
Minus 3/8 inch (10 mm).d. Each additional 10 feet (3 m), Plus or
Minus 1/8 inch (3 mm).
3. Total Thickness or Flange Thickness: Plus _ inch (6 mm),
Minus 1/8 inch (3 mm).4. Rib Thickness: Plus or Minus 1/8 inch (3
mm).5. Rib to Edge of Flange: Plus or Minus 1/8 inch (3 mm).6.
Distance between Ribs: Plus or Minus 1/8 inch (3 mm).7. Variation
from Square or Designated Skew (Difference in Length of the Two
Diagonal 8. Measurements): Plus or Minus 1/8 inch per 72 inches (3
mm per 2 m) or 1/2 inch (13 mm) total,
whichever is greater.
8. Length and Width of Block-outs and Openings within One Unit:
Plus or Minus 1/4 inch (6 mm).9. Location and Dimension of
Block-outs Hidden from View and Used for HVAC and Utility
Penetrations: Plus or Minus 3/4 inch (19 mm).10. Dimensions of
Haunches: Plus or Minus 1/4 inch (6 mm).11. Haunch Bearing Surface
Deviation from Specified Plane: Plus or Minus 1/8 inch (3 mm).12
Difference in Relative Position of Adjacent Haunch Bearing Surfaces
from Specified Relative Position: Plus or Minus 1/4 inch (6 mm).13.
Bowing: Plus or Minus L/360, maximum 1 inch (25 mm).14. Local
Smoothness: 1/4 inch per 10 feet (6 mm per 3 m).15. Warping: 1/16
inch per 12 inches (1.5 mm per 300 mm) of distance from the nearest
adjacent corner.16. Tipping and Flushness of Plates: Plus or Minus
1/4 inch (6 mm).17. Dimensions of Architectural Features and
Rustications: Plus or Minus 1/8 inch (3 mm).
C. Position Tolerances: For cast-in items measured from datum
line location, as indicated on Shop Drawings.
1. Weld Plates: Plus or Minus 1 inch (25 mm).2. Inserts: Plus or
Minus 1/2 inch (13 mm).3. Handling Devices: Plus or Minus 3 inches
(75 mm).4. Reinforcing Steel and Welded Wire Reinforcement: Plus or
Minus 1/4 inch (6 mm) where position has structural implications or
affects concrete cover; otherwise, Plus or Minus 1/2 inch (13
mm).5. Reinforcing Steel Extending out of Member: Plus or Minus 1/2
inch (13 mm) of plan dimensions.6. Tendons: Plus or Minus 1/4 inch
(6 mm), vertical; Plus or Minus 1 inch (25 mm), horizontal.7.
Location of Rustication Joints: Plus or Minus 1/8 inch (3 mm).8.
Location of Opening within Panel: Plus or Minus 1/4 inch (6 mm).9.
Location of Flashing Reglets: Plus or Minus 1/4 inch (6 mm).10.
Location of Flashing Reglets at Edge of Panel: Plus or Minus 1/8
inch (3 mm).11. Reglets for Glazing Gaskets: Plus or Minus 1/8 inch
(3 mm).12. Electrical Outlets, Hose Bibs: Plus or Minus 1/2 inch
(13 mm).13. Location of Bearing surface from End of Member: Plus or
Minus 1/4 inch (6 mm).14. Allowable Rotation of Plate, Channel
Inserts, Electrical Boxes: 2-degree rotation or 1/4 inch (6 mm)
maximum over the full dimension of the unit.15. Position of Sleeve:
Plus or Minus 1/2 inch (13 mm).16. Location of Window Washer Track
or Buttons: Plus or Minus 1/8 inch (3 mm).
Delete paragraph below if brick faced architectural units are
not used. The number of bricks allowedthese misalignments should be
limited to 2 percent of the bricks on the unit.
D. Brick-Faced Architectural Precast Concrete Units. 1.
Alignment of mortar joints:
a. Jog in Alignment: 1/8 inch (3 mm).b. Alignment with Panel
Centerline: Plus or Minus 1/8 inch (3 mm).
2. Variation in Width of Exposed Mortar Joints: Plus or Minus
1/8 inch (9 mm).3. Tipping of Individual Bricks from the Panel
Plane of Exposed Brick Surface: Plus 1/16 inch (1.5 mm); Minus 1/4
inch (6 mm) < depth of form liner joint.
4. Exposed Brick Surface Parallel to Primary Control Surface of
Panel: Plus 1/4 inch (6 mm); Minus 1/8 inch (3 mm).5. Individual
Brick Step in Face from Panel Plane of Exposed Brick Surface: Plus
1/16 inch (1.5mm); Minus 1/4 inch (6 mm) < depth of form liner
E. Stone Veneer-Faced Architectural Precast Concrete Units.
Tolerances below are generally appropriate for smooth-finished
stone. Retain, delete, or revise to suitProject.
1. Variation in Cross-Sectional Dimensions: For thickness of
walls from dimensions indicated: Plus or Minus 1/4 inch (6 mm).2.
Variation in Joint Width: 1/8 inch in 36 inches (3 mm in 900 mm) or
a quarter of nominal joint width, whichever is less.
Revise or delete below for natural-cleft, thermal, and similar
3. Variation in Plane between Adjacent Stone Units (Lipping):
1/16 inch (1.5-mm) difference between planes of adjacent units.
A. Panel faces shall be free of joint marks, grain, and other
obvious defects. Corners, including falsejoints shall be uniform,
straight and sharp. Finish exposed-face surfaces of architectural
precastconcrete units to match approved [design reference sample]
[sample panels] [mockups] and asfollows:
This Article presumes Architect has preapproved one or more
design reference samples. Includecomplete description of design
reference sample here. If preapproving manufacturers, coordinate
withManufacturers Article. Revise if multiple samples are
1. Design Reference Sample:
Delete subparagraph below if not used. PCI published numbered,
color photographs of 428 precastconcrete finishes, see PCIs website
www.pci.org. Revise below and add reference number. Addreference
number combinations if more than one finish is required.
2. PCIs Architectural Precast Concrete Color and Texture
Selection Guide, of plate numbersindicated.
Retain type of finish from subparagraphs below if needed. If
more than one finish is required, addlocations to finish
descriptions or indicate on Drawings. Add more detailed
descriptions of finishesoutlined below if required when greater
definition is required, such as (light), (medium), or (deep).Remove
matrix to a maximum depth of one-third the average diameter of
coarse aggregate but not morethan one-half the diameter of smallest
sized coarse aggregate. See PCI MNL 117 for more informationon
finishes. An as-cast finish generally results in a mottled surface
or non-uniform finish.
on finishes. An as-cast finish generally results in a mottled
surface or non-uniform finish.
3. As-Cast Surface Finish: Provide surfaces free of excessive
air voids, sand streaks, andhoneycombs.
4. Textured-Surface Finish: Impart by form liners to provide
surfaces free of excessive air voids,sand streaks, and honeycombs,
with uniform color and texture.
5. Bushhammer Finish: Use power and hand tools to remove matrix
and fracture coarse aggregates.6. Exposed Aggregate Finish: Use
chemical retarding agents applied to concrete forms and
washing and brushing procedures to expose aggregate and
surrounding matrix surfaces after formremoval.
7. Abrasive-Blast Finish: Use abrasive grit, equipment,
application techniques, and cleaningprocedures to expose aggregate
and surrounding matrix surfaces.
8. Acid-Etched Finish: Use acid and hot-water solution,
equipment, application techniques, andcleaning procedures to expose
aggregate and surrounding matrix surfaces. Protect
hardware,connections and insulation from acid attack.
9. Honed Finish: Use continuous mechanical abrasion with fine
grit, followed by filling andrubbing procedures.
10. Polished Finish: Use continuous mechanical abrasion with
fine grit, followed by filling andrubbing procedures.
11. Sand-Embedment Finish: Use selected stones placed in a sand
bed in bottom of mold, with sandremoved after curing.
B. Finish exposed [top] [bottom] [back] surfaces of
architectural precast concrete units to match face-surface
Retain paragraph above or below if applicable. Revise below to
float finish or light-broom finish ifsmooth, steel-trowel finish is
C. Finish unexposed surfaces [top] [bottom] [and back] of
architectural precast concrete units bysmooth steel-trowel
Revise finish below to light-broom, stippled, or as-cast finish
if float finish is unnecessary, orupgrade to smooth, steel-trowel
D. Finish unexposed surfaces of architectural precast concrete
units by float finish.
2.21 SOURCE QUALITY CONTROL
Always retain paragraph below because it establishes the minimum
standard of plant testing andinspecting. PCI MNL 117 mandates
source testing requirements and a plant Quality Systems Manual.PCI
certification also ensures periodic auditing of plants for
compliance with requirements in PCIMNL 117.
A. Quality-Control Testing: Test and inspect precast concrete
according to PCI MNL 117 requirements.If using self-consolidating
concrete also test and inspect according to PCI Interim Guidelines
for theUse of Self-Consolidating Concrete.
Delete paragraph and subparagraph below if not required. PCI
certification would normally beacceptable to authorities having
jurisdiction without further monitoring of plant quality-control
andtesting program by Owner.
B. Owner will employ an independent testing agency to verify
architectural precast concrete fabricatorsquality-control and
1. Allow Owners testing agency access to material storage areas,
concrete production equipment,concrete placement, and curing
facilities. Cooperate with Owners testing agency and providesamples
of materials and concrete mixes as may be requested for additional
C. Strength of precast concrete units will be considered
deficient if units fail to comply with ACI 318(ACI 318M)
requirements for concrete strength.
Review testing and acceptance criteria with structural engineer.
Add criteria for load tests if required.
D. Testing: If there is evidence that the concrete strength of
precast concrete units may be deficient ormay not comply with ACI
318 (ACI 318M) requirements, Precaster will employ an
independenttesting agency to obtain, prepare, and test cores
drilled from hardened concrete to determinecompressive strength
according to ASTM C 42/C42M.1. A minimum of three representative
cores will be taken from units of suspect strength, from
locations directed by Architect.2. Cores will be tested in an
PCIs recommendations below are more stringent than ACIs.
3. Strength of concrete for each series of 3 cores will be
considered satisfactory if the averagecompressive strength is equal
to at least 85 percent of the 28-day design compressive strengthand
no single core is less than 75 percent of the 28-day design
4. Test results will be made in writing on the same day that
tests are performed, with copies toArchitect, Contractor, and
precast concrete fabricator. Test reports will include the
following:a. Project identification name and number.b. Date when
tests were performed.c. Name of precast concrete fabricator.d. Name
of concrete testing agency.e. Identification letter, name, and type
of precast concrete units or units represented by core
tests; design compressive strength; type of break; compressive
strength at breaks, correctedfor length-diameter ratio; and
direction of applied load to core in relation to horizontal planeof
concrete as placed.
E. Patching: If core test results are satisfactory and precast
concrete units comply with requirements,clean and dampen core holes
and solidly fill with precast concrete mix that has no coarse
aggregate,and finish to match adjacent precast concrete
F. Defective Work: Architectural precast concrete units that do
not comply with acceptability
requirements in PCI MNL 117, including concrete strength,
manufacturing tolerances, and color andtexture range are
unacceptable. Chipped, spalled or cracked units may be repaired, if
repaired unitsmatch the visual mock-up. The Architect reserves the
right to reject any unit if it does not match theaccepted samples
and visual mock-up. Replace unacceptable units with precast
concrete units thatcomply with requirements.
PART 3 EXECUTION
A. Deliver anchorage devices that are embedded in or attached to
the building structural frame orfoundation before start of such
work. Provide locations, setting diagrams, and templates for
theproper installation of each anchorage device.
A. Examine supporting structural frame or foundation and
conditions for compliance withrequirements for installation
tolerances, true and level bearing surfaces, and other
conditionsaffecting performance. Proceed with installation only
after unsatisfactory conditions have beencorrected.
B. Do not install precast concrete units until supporting
cast-in place concrete building structuralframing has attained
minimum allowable design compressive strength or supporting steel
or otherstructure is structurally ready to receive loads from
A. Install loose clips, hangers, bearing pads and other
accessories required for connecting architecturalprecast concrete
units to supporting members and backup materials.
B. Erect architectural precast concrete level, plumb and square
within the specified allowabletolerances. Provide temporary
supports and bracing as required to maintain position, stability,
andalignment of units until permanent connections are
1. Install temporary steel or plastic spacing shims or bearing
pads as precast concrete units arebeing erected. Tack weld steel
shims to each other to prevent shims from separating.
2. Maintain horizontal and vertical joint alignment and uniform
joint width as erection progresses.3. Remove projecting lifting
devices and use sand-cement grout to fill voids within recessed
lifting devices flush with surface of adjacent precast concrete
surfaces when recess is exposed.4. Unless otherwise shown provide
for uniform joint widths of 3/4 inch (19mm)
C. Connect architectural precast concrete units in position by
bolting, welding, grouting, or asotherwise indicated on approved
Erection Drawings. Remove temporary shims, wedges, andspacers as
soon as practical after connecting and/or grouting are
1. Disruption of roof flashing continuity by connections is not
permitted; concealment within roof insulation is acceptable.
D. Welding: Comply with applicable AWS D1.1 and AWS D1.4
requirements for welding, weldingelectrodes, appearance, quality of
welds, and methods used in correcting welding work.
1. Protect architectural precast concrete units and bearing pads
from damage by field welding orcutting operations and provide
noncombustible shields as required.
2. Welds not specified shall be continuous fillet welds, using
not less than the minimum fillet asspecified by AWS.
3. Clean weld affected metal surfaces with chipping hammer
followed by brushing then apply aminimum 0.004 inch (100 _m) thick
coat of galvanized repair paint to galvanized surfaces
inconformance with ASTM A780.
Retain subparagraph above or below.
4. Clean weld affected metal surfaces with chipping hammer
followed by brushing then reprimedamaged painted surfaces in
accordance with manufacturers recommendations.
5. Visually inspect all welds critical to precast connections.
Visually check all welds forcompletion and remove, reweld or repair
all defective welds, if services of AWS-certifiedwelding inspector
are not furnished by Owner.
E. At bolted connections, use lock washers, tack welding, or
other acceptable means to preventloosening of nuts after final
1. Where slotted connections are used, verify bolt position and
tightness. For sliding connections,properly secure bolt but allow
bolt to move within connection slot. For friction connectionapply
specified bolt torque and check 25 percent of bolts at random by
Revise locations and extent of grouting in paragraph below if
F. Grouting Connections: Grout connections where required or
indicated. Retain grout in place untilhard enough to support
itself. Pack spaces with stiff grout material, tamping until voids
arecompletely filled. Place grout to finish smooth, level, and
plumb with adjacent concrete surfaces.Promptly remove grout
material from exposed surfaces before it affects finishes or
3.4 ERECTION TOLERANCES
A. Erect architectural precast concrete units level, plumb,
square, true, and in alignment withoutexceeding the noncumulative
erection tolerances of PCI MNL 117, Appendix I.
Select paragraph above or paragraph and subparagraphs below.
Usually retain above unlesstolerances for Project deviate from PCI
recommendations. PCI MNL 117 erection tolerances arelisted below.
If more exacting tolerances are required for Project, coordinate
with fabricationtolerances for precast concrete as well as erection
tolerances for supporting construction.
B. Erect architectural precast concrete units level, plumb,
square, and true, without exceeding thefollowing noncumulative
1. Plan Location from Building Grid Datum: Plus or Minus 1/2
inch (13 mm).2. Plan Location from Centerline of Steel: Plus or
Minus 1/2 inch (13 mm).3. Top Elevation from Nominal Top Elevation:
a. Exposed Individual Panel: Plus or Minus 1/4 inch (6 mm).b.
Nonexposed Individual Panel: Plus or Minus 1/2 inch (13 mm).c.
Exposed Panel Relative to Adjacent Panel: 1/4 inch (6 mm).d.
Nonexposed Panel Relative to Adjacent Panel: 1/2 inch (13 mm).
4. Support Elevation from Nominal Support Elevation: As
follows:a. Maximum Low: 1/2 inch (13 mm).5. Maximum High: 1/4 inch
5. Maximum Plumb Variation over the Lesser of Height of
Structure or 100 Feet (30 m): 1 inch(25 mm).
6. Plumb in Any 10 Feet (3 m) of Element Height: 1/4 inch (6
mm).7. Maximum Jog in Alignment of Matching Edges: 1/4 inch (6
mm).8. Joint width (Governs over Joint Taper): Plus or Minus 1/4
inch (6mm).9. Maximum Joint Taper: 3/8 inch (10 mm).10. Joint Taper
in 10 Feet (3 m): 1/4 inch (6 mm).11. Maximum Jog in Alignment of
Matching Faces: 1/4 inch (6 mm).12. Differential Bowing or Camber,
as Erected, between Adjacent Members of Same Design: 1/4
inch (6 mm).13. Opening Height between Spandrels: Plus or Minus
1/4 inch ( 6 mm).
3.5 FIELD QUALITY CONTROL
Retain this Article if field testing and inspecting are
required. Revise paragraph below if Contractorengages agency.
A. Testing: Owner will engage a qualified independent testing
and inspecting agency to perform fieldtests and inspections.
B. Field welds will be subject to visual inspections and
non-destructive testing in accordance withASTM E165 or ASTM
C. Testing agency will report test results promptly and in
writing to Contractor and Architect.
D. Repair or remove and replace work that does not comply with
E. Additional testing and inspecting, at Contractors expense,
will be performed to determinecompliance of corrected work with
Blemishes occurring after delivery are normally repaired before
final joint sealing and cleaning asweather permits.
A. Repairs will be permitted provided structural adequacy of
units and appearance are not impaired.
The precast concrete manufacturer should develop appropriate
repair mixtures and techniques duringthe production sample approval
B. Mix patching materials and repair units so cured patches
blend with color, texture, and uniformityof adjacent exposed
surfaces and show no apparent line of demarcation between original